Resins for Surface Coatings Vol 2
Download Resins for Surface Coatings Vol 2...
RESINS FOR SURFACE COATINGS
Volume II (SecondEdition)
Alkyds & Polyesters by P Deligny N Tuck Edited by PKT Oldring
JOHN WILEY AND SONS CHICHESTER – NEW YORK – WEINHEIM – TORONTO – SINGAPORE
Published in association with
SITA TECNOLOGY LIMITED LONDON UK
Resins for Surface Coatings
VOLUME II Alkyds & Polyesters
P. Deligny N. Tuck Edited by PKT Oldring
Since the 1980's there have been many significant changes in surface coatings which have necessitated major changes in the resins used, even though many may still be referred to by generic names. Thus it is appropriate that a series of books written for graduates new to the resins and surface coatings industries, which became recognised globally as an overview of the technology of resins for surface coatings should be revised and issued in time for the new millennium to reflect the recent advances within these industries, whilst retaining the basic understanding for which this original series of books was renowned. It is reported that there was a time when the surface coatings industry dealt with a relatively small number of materials and processes for making paints and varnishes. Indeed it is claimed that between 1736 and 1900, Watin's book on varnish formulations was reprinted 14 times with only minor modifications. This was claimed(4) to be the industry standard. Compare that with today's situation. A book which lasts for 200 years to the turn of the century, followed by a series of books) published in the 1940's which last 40 years to be superseded by a set which lasts 20 years before needing to undergo major revisions. It is not the writing which is inadequate, but it is a true reflection of the increasing rate of change of the surface coating industry. Reference to some of the earlier text books written for the surface coatings industry reveal how far this industry has progressed over the last 50 or so years. Examination. of a 5 volume set of books published by Wiley will be used to illustrate the changes and progress which have occurred and the approximate dates for introduction of what were considered new technologies over the last hundred or so years. Dates for new technology developments may be the Aject of debate, because it was often different between North America and Europe and even within some parts of Europe. Dates are given to try and put this industry and its developments into perspective. In the early 1900's resins used for surface coatings were based upon naturally occurring materials, albeit with some degree of modification or processing in some cases. Some of the early resins for surface coatings resembled alchemy, with secret ingredients and/or processing techniques being handed down from father to son (at the turn of the century, there were few female resin chemists). In the opening paragraph of Volume III, Chapter 4 of Mattelio's book written in the early 1940's as reproduced here, the reader will note a lot of similarities to the above paragraph and some would question if the situation had changed. Rest assured it has changed beyond all recognition from. the 1940's let alone prior to 1900! "The art and skill of the old-time varnish maker have yielded slowly-to more scientific control and to the developments of the chemists and engineers who have entered the
coating-materials industries. The complexity of the organic: molecules which they have had to deal with, however, has necessitated the continued use of methods which, although wore exact and more scientifically grounded than those of their predecessors, nevertheless are still quite empirical. “it is well to remember that the molecular complexity of the drying oils and resins which are now (1943) in commercial use has provided a formidable variety of problems, which have long proved perplexing... Under such circumstances, one hardly need wonder that empiricism has so long prevailed or why there have been so many recorded differences of opinion and conflicting experimental observations". To quote a recognised industry standard publication 55 years ago, “manufacture was in the hands of untrained men. Chemists or engineers, if there were any in this industry one hundred years ago (ca 1850), were a curiosity. The breadth of science had not yet touched it, and most manufacturers at that time saw no reason why it should” When resins were processed, early controls consisted of mainly empirical factory, such as string length - how long a piece of resin could be stretched before breaking. The objective was to process a resin as close to its 'gel point', without actually gelling. Much thermal processing was on gas fired open iron vessels, which resembled a pan on a gas cooking ring. Foam over and associated fires were common place. Indeed, folklore has it that some resin processing was controlled by processing until it "foamed over" or ignited. Early surface coatings were limited to mainly air drying systems which film formed by either evaporation of solvent, to leave a dried film of the natural resin or oxidative cross-linking of any unsaturation present in vegetable oil based binders. French polish, based upon shellac is an example of the first type of coating, whilst alkyds or oleo-resinous based systems are examples of the latter. Alkyds and oleo-resinous based coatings were originally used for many surface coating applications, where there was a performance demand, such as increased durability or resistance to water or alkali, compared to alterative systems. The unsaturation in the vegetable oil portion of the resin enabled cross-linking reactions, induced by oxygen in the air, to form resistant and durable films. Some decorative paints, based on linseed oil, for example, could easily yellow. Other systems (varnishes, rather than coatings), were often based upon solutions of hard, naturally occurring resins. Today coatings can be divided into thermoplastic and thermo-set. Thermoplastic systems primarily film form by evaporation of solvent. As a general rule, thermoplastics coatings are based on high molecular weight polymers. solutions of high molecular weight thermoplastic resins are normally too high in viscosity for the desired applications solids, hence dispersions of thermoplastic resins are frequently used. A dispersion in water, maybe an acrylic latex or emulsion, typically used in home decorative emulsion wall paints.
Thermoplastic polymers may also be dispersed in organic solvents, although the solvent is not a solvent for the polymer. An example would be a dispersion of PVC in organic solvents, commonly known as an organo-sol. Organo-sol coatings are used for architectural coil for claddings and the internal coatings, mainly coil applied, of easy open ends for beer and beverage cans. Another approach to obtaining a resistant film of high molecular weight, whilst having good application solids viscosity relationships is to use thermo-set systems. Here relatively low molecular weight resins with chemical functionality. Being of low molecular weight, they give relatively low viscosity at the required application solids. Film formulation is induced by either mixing the two components, as in a two pack epoxy, polyamine heavy duty coating, or by the application of heat to a one pack epoxy phenolic can coating. The stability of a thermoset coating, once mixed, is of great importance. Should chemical reaction be prematurely induced, then the viscosity could rapidly and easily increase to a point where the coating is unusable. For one pack coatings the unusable period is referred to as die shelf life, normally measured in months, whilst for two pack coatings it is the pot life, normally measured in hours. Protective coatings have been used for many years. They are no restricted to industrial coatings and include house paints, because the paint or varnish protected die wooden parts of the house. Varnishes are also covered by the term 'protective coatings', because vanishes, such as spar varnishes, protect the spars on sailing ships. Not only were die paints and varnishes derived from vegetable oils and natural materials, many of which have disappeared, but they were classified in a way which few resin and paint chemists would recognise today, particularly if they are relatively new to this industry. Varnishes in the past were divided into two types, with many sub-divisions, as follows: Oleo-resinous varnishes
Oil plus natural resins Oil plus synthetic resin Oil Oil modified glycerol phthalate Oil modified chlorinated rubber
Solvent plus natural resins Solvent plus synthetic resins
The first group dry by oxidation or process initiated by oxidation, whilst he second dry by evaporation.
Before 1905 house paints consisted of white lead, linseed oil, driers and thinners (solvent). Later, zinc: oxide was used at about 20-30% of the pigment by weight. Extenders, such as barites and magnesium silicate, only started to be used from about 1910 onwards. A red lead primer was often used for metal structures, such as bridges. The mid 1900's saw a rise in the use of aluminium top coats for metal structures. Lacquers referred to certain natural products used in the Chinese and Japanese or solutions of resinous materials in volatile solvents. However, this term also came to cover solutions of nitrocellulose. These became of great importance to the automobile industry in the 1920's, seeking a faster finish than that obtainable for oleo-resinous materials. The commercial availability of ketonic: and ester solvents greatly assisted the market penetration of nitrocellulose lacquers. These lacquers came to also be used on furniture. However, due to its brittle nature, nitrocellulose films needed plasticizing. Alkyds were developed for this purpose and the resulting properties of an alkyd nitrocellulose film were beneficial. Some of the natural resins used in the protective surface coatings industry in the past were dammar, kauri, copal, congo, east india, zanzibar, sandarac, manila and amber. As the name suggest, they often reflected their geographic origin. Natural resins were often 'run' to impart oil solubility. This involved heating to some extent to depolymerise the resin. Weight losses up to 30% could occur and the process generated copious fumes. With synthetic resins, such as phenolics, polymerisation occurs. Spirit varnishes used lacs, which are of insect origin. It has been estimated that 1,500,000 insects are required to produce sufficient: lac for 0.5 kg of shellac. The use of natural resins has decreased in the USA since about 1930, with them being replaced by synthetic resins. Rosin was, and is, an important member of this family. It is used in the preparation of both varnishes and synthetic resins and as such its usage did no drop to the same extent as other natural resins. Rosin is used to form ester gums, which are based upon the glycerol reaction with rosin, plus other components in many cases. In 1938, 61% of linseed oil consumption was for paints and varnishes. Other uses included linoleum, oil cloth, printing and patent leather. Certainly at this time as in days before, linseed oil was of major importance to the surface coatings industry. Linseed oil was subdivided into numerous types depending upon its processing. Some of these were raw linseed oil, alkali refined linseed oil, acid refined linseed oil, oxidised linseed oil, heat bodied drying oils, air bodied versus vacuum bodied. Linseed oil was normally prebodied before combination with natural resins, whilst this was not needed for tung oil. Tung oil was first imported into the USA about 1870. It took time for formulators to learn how to process the oil to avoid the problems of wrinkling, crow's feet, rapid bodying or onset of gelation and matt appearance. Between 1915 and 1925, varnish making was adapted to utilise this new material by gas-checking the oil, which involved heating it to 500'F. Many of the varnishes used 90% tung oil and 10% Linseed oil(4). Phenolic resins had a major impact on the use of tung oil. Perilla oil, which has similar properties to those of linseed oil, with faster drying and harder films, only came into importance during the 1030's. It was often used m combination with tung oil (75% tung and 25% perilla) and alone in alkyds.
Otocacia oil was first used in about 1923 and was believed to be similar to tung oil, but later this was found not to be the case, being inferior in water and lacking alkali resistance and with behaviour more like that of a resin than an oil causing embitterment However, by modification of the resins used with this oil, it could be used as a replacement for tung oil. Ester gums based on this oil have also been prepared. Castor oil, not being a drying oil, was used as a plasticizer for lacquers. Whilst the dehydration of this oil was the subject of Much study over many years, it was not until about 1937 to 1939(4-6) that dehydrated castor oil (DCO) became commercially available. Even then, it was only 75 to ~M% dehydrated, which gave rise to a tackiness in the dried films. By late 1938, 95% to 98% dehydrated castor oil was available, and many of the earlier obstacles and objections to the use of this oil were overcome. Bodying the oil under vacuum gave low acid value stand oils, which could be used to replace, fully or partially, tung oil. Soybean oil was unknown in 1909 as a raw material for paints and varnishes. It became an important oil in the mid-1930's. It was used for non-yellowing, white baking enamels. When fortified with tung oil, alkyd resins suitable for automotive finishes were obtained. Combination with phenolic: resins also gave acceptable varnishes. Fish oils, such as sardine oil, have been used, but today this practice has virtually ceased. Odour and variable composition of the oils were two main reasons, with availability as fish stocks decline being an additional one. Synthetic resins used in the middle of the 20 century included: Ester gums, based upon reaction of rosin with glycerol or other polyhydric alcohols, were used from about 1900 onwards, and were important raw materials. Nowadays their use is limited. Other natural resins, such as copal, were sometimes used to produce ester gums. Coumarone indene resins were in commercial production in the USA before 1920 and as such could be considered as the first commercially available synthetic resins. They impart alkali, acid and brine resistance, good adhesion and fast drying. They were also used in combination with phenolic resins. The reaction of phenol with aldehydes was documented in 1872. Phenolic resins have been used commercially since about 1916 in Europe, and in 1922 in the USA. Many of the phenolic resins used today would bear little resemblance to the early phenolic resins. They were primarily based upon phenol and formaldehyde. It was not until about 1926 that intensive developments of modified phenolic: resins got underway in earnest. In 1931 p-ter-butylphenol and p-phenylphenol based phenolic resins were introduced, whilst 1937 saw the use of bisphenol A in phenolic resins. Many of these modifications were brought about by attempts to improve the oil solubility of the phenolic resins. Reaction of modified phenolic resins with rosin or copal made the resulting product oil-soluble. Modification of phenolic resins with ester gums was common practice. Fast drying times of touch dry within 4 hours were achieved. Tung oil varnishes modified with phenolic resins gave vastly improved water and alkali resistance finishes. Even when modified with ester gums, significantly improved water and alkali resistance was obtained compared with that from natural resin based varnishes.
It has been known since 1901 that phthalic anhydride reacts with glycerol, a by-product of refining oils (triglycerides) to form fatty acids. This was the foreigner to the largest class of synthetic resins which are still in use today, namely alkyds. They are based upon oils or fatty acids with polyhydric alcohols, such as glycerol or pentaerythritol, and polybasic acids such as phthalic anhydride. In addition, monofunctional acids or alcohols may also be present Initially, drying oils or fatty acids were used for baking or air-drying finishes. In 1929, differentiation between air (oxygen) and heat convertible alkyds was made. Alkyds have been a major resin in the surface coatings industry since about 1928-1930. Automobile finishes (enamels) were based upon alkyd resins, even though they required baking at higher temperatures than the alterative nitrocellulose lacquers. Even nitrocellulose based automotive lacquers contained a proportion of alkyd resin. Due to the final properties of the alkyd, the complexity of combinations of type of oil or fatty acid and other components and the various ways of processing, a generation of alkyd chemists emerged. Polyvinyl acetate was the first important vinyl resin and was available in about 1912. Aldehyde treated polyvinyl acetate resins were used for spirit type varnishes, lacquers and enamels which has good weathering properties. Some of the higher aldehyde modified polyvinyl acetates gave good baking varnishes. Copolymers of vinyl acetate and vinyl chloride then became available. They tended to be more used in Europe, whilst the USA tended to use polyvinyl chloride resins for surface coatings. One reason was the rubber-like characteristics of polyvinyl chloride. Indeed, it was used as a rubber substitute. Acrylic resins were first used in surface coatings in about, 1935. Since this time, hundreds of different acrylic based resins have been made commercially available, with a wide range of characteristics. Many in the coatings industry tend to consider styrene as an acrylic comonomer Polystyrene is claimed 61 to be the oldest synthetic resin, having been 'discovered' about 1800. They are commercially available in Europe in the 1920's and it was not until the late 1930's that they were produced in the USA Chlorinated rubber is soluble in many solvents and has good compatibility with many materials used in paints. It imparts alkali and moisture resistance to films containing it. Chlorinated rubber resins were used in the USA from about 1934 onwards, having been used in Europe for a few years before. Urea formaldehyde resins, which are part of the aminoplast family, and their use with alkyd resins were reported in about 1930. Applications reported in the 1940's included metallic articles requiring resistance to adverse conditions, whilst retaining good appearance, of which automobiles, refrigerators and bicycles were three such examples. In 1945 it was stated that the era of urea formaldehyde resins as coasting materials was just beginning. Viewed from today's perspective, this was a very apt vision, especially when one considers the other aminoplast resins now available which complement the early urea formaldehyde resins. Melamine formaldehyde resins started to become available from about 1940 onwards. These materials are co-curing resins, which means that in addition to film forming themselves they can crosslink with other resins containing functional groups, such as hydroxylic groups in alkyds, polyesters, epoxies and acrylics, acidic groups in alkyds, polyesters and acrylics, epoxy groups m epoxy resins and amine groups in acrylics. Phenolic resins can also be considered as co-cure resins.
Epoxies resins only became commercially available in about 1947. Since then their usage has grown to over 550,000 tonnes per year (1990), but all are not for coating applications. They impart outstanding resistance properties and find many applications, including 1 and 2 pack air drying systems. The latter includes, the polyamine, polyamide or polyamino-amide heavy duty coatings, where the amine functionality cross~ the epoxy resin to give a durable and resistant film They are typically used for marine applications such as ship's hulls,-decks, superstructure and tanks, oil rigs and other off-shore installations, storage tanks for food, chemicals and water, pipe linings and paints for concrete and cement. Heat cured coatings based on epoxy resins are used for can linings or internal lacquers, automotive primers and powder coatings. Epoxy resins can be reacted with other materials to improve the performance of either. There are two types of epoxy esters. One is for air drying coatings and the other is for stoved ones. For air drying epoxy esters, epoxy resin is reacted with air drying oils or fatty acids. For good colour retention, fatty acids with low degrees of unsaturation, such as coconut, would be reacted with the epoxy resin/ film formation would be through cross-linking, probably through the use of an aminoplast. Polyurethanes did not gain any prominence in surface coatings until he latter half of the 20 Century. Based upon isocyanates and hydroxyl functional materials, a wide range of properties could be attained. Additionally, isocyanates are used to crosslink resins. In he period 1930-1940, pigments consisted of white lead, basic lead sulphate, litharge, red lead, zinc oxide, leaded zinc, lithopone and blanc fixe. Titanium dioxide started to become commercially available in about 1918 and even in 1943 it was stated(41 that the tonnage consumed by the paint industry had grown considerably. High opacity rutile titanium dioxide was available from 1941. It had superior exterior durability and hiding power compared to anatase titanium dioxide. Synthetic: organic pigments which had a usable level of light-fastness were made possible in 1914, when it was realised that reaction of the dyes with complex inorganic acids imparted such properties. Phthalocyanine based pigments came into being about 1927. For air drying oils or fatty acids to dry efficiently, it was normal practice to add 'driers' which were mainly based upon lead, manganese and cobalt. They were often used in the form of naphthenates or linoleates. Today, whilst driers are still required they are based upon less toxic metals such as calcium, barium or zinc. As the demands on surface coatings increased, and as the complexity of the resins needed to meet these demands also increased, so the resin raw materials and processing techniques changed out of all recognition. Some of the earliest modem resin process controls used 'wet chemistry' techniques such as acid value in conjunction with solids (non-volatile content - NVQ and viscosity measurements. By plotting acid value against viscosity during the process it was (and is) possible to safely continue a reaction to close to the 'gel point', without gelation. This approach also ensured a greater degree of reproducibility. In essence, the monitoring of acid value and viscosity for alkyds and polyesters, was a means of controlling the molecular weight of the resin. With analytical techniques rapidly improving, it is now possible to routinely monitor molecular weights using Gel Permeation Chromatography (GPC).
Improvements in Spectroscopy, such as Fourier Transform Infra Red (FTIR), enables rapid checking of quality of either raw materials or finished products. The area of Statistical Process Control (SPC) is now commonplace in resin and coating manufacture. As the requirements for coatings increase and formulations have to balance numerous opposing properties, the need for consistency of product becomes more important. In the early days the quality of the raw materials could be variable, to say the least. With many being based on naturally occurring materials, their composition could vary due to variable climatic conditions during the growing season(s) or geographic region(s). This is true of some of these materials even today. For example, the compositions of North American and Scandinavian tall oil fatty acids, which are derived from the stumps of trees, is different. For some applications this doesn't matter, but for other more sensitive ones, this difference can exclude the use of tall oil fatty acid from a particular source. With ever improving analytical techniques and understanding of the science of processing of raw materials, variations in composition are now much reduced. Raw material innovations and developments have been fundamental for the development of resins and coatings with improved performance, lower cost and improved environmental acceptability. The more sophisticated the raw materials, the greater the process control necessary and the better the product consistency. Initially, most coatings were solvent based, many of low solids content. With environmental pressures, there has been a move towards waterborne or high solids content systems. However, many waterborne systems still contain organic solvent. Additionally, neutralising amine is also present. Both solvent borne and water borne systems have to meet VOC (volatile organic compounds) legislation. The applicators and users of coatings have the option of incineration of solvent or waterborne to reduce their emissions of organic materials. However, it has to be borne in mind that incineration of solvent whilst reducing the fuel costs of the incinerator will increase the emissions of carbon dioxide, which has the potential for being the subject of a future tax for some European countries. However, with the environmental requirement of some countries, it may be necessary to continue to incinerate to comply with 'odour' emissions at the boundary fences of the factory site, even for waterborne systems. Hence there will. be the balance of costs of incinerator fuel verses calorific value of solvent versus size of incinerator - incineration of a waterborne system requires a much smaller incinerator that that for an equivalent volume of solvent based coatings. Before the Second World War many surface coatings were based on-alkyds. The rate of change in the last 40 years is truly remarkable. The demise of alkyds has been predicted many times, but the fact that they are still a major class of surface coating resin is a tribute to their versatility. Alkyds have been modified to suit the demands placed upon them. Today waterborne and high solids alkyds are commonplace. Twenty or so years ago, these alkyd technologies were in their infancy. It would take a brave person wagering against the alkyd technology continuing for another 100 years due to the ability to relatively easily modify them and the face that they are based upon the renewable raw materials (vegetable oils) and are extremely cost competitive. Many of the traditional areas of surface coating will continue with modifications to suit external pressures.
Heavy duty coatings will continue to be, for the main part, based upon epoxy polyamine/polyamide technology. For certain applications, waterborne heavy duty coatings are commonly used as are some solvent-less systems. One of the reasons for the continued use of tried and trusted technologies, is the fact that they are tried and trusted. In the case of heavy duty and many industrial coatings, the cost of the coating is small compared to the article being coated, and normally results in an enhanced value or prolonged lifetime of the article. Thus, the fabricators of articles and applicators of coatings tend to be conservative and use tried and trusted coatings, albeit with modifications to suit environmental or other concerns. The can coating business, with its use of epoxy phenolic internal lacquers, is another example of tried and trusted technology surviving. In some areas, however, there have been dramatic changes in the coating technologies used. One such example would be "white goods" which are domestic appliances such as washing machines and refrigerators. This market is now predominantly powder coating, whereas a few years ago acrylic technology dominated. The automotive market is another which has seen 'leaps' of technology. Electro deposition, initially anodic and now cathodic, dominates for automotive primers. Some areas have seen rapid adoption of what were considered at the time as radical technologies, with powder coatings and radiation curable being two good examples. Both of these technologies whilst being solvent free, are unable to meet all of the demands of the end applications. Hence, there is and will continue to be a place for liquid solvent based or waterborne coatings, even if major modifications are required to enable them to meet environmental legislation. In some cases, such as wood coatings. geographic preferences dictate the technology used. The choices are alkyd aminoplast or radiation curable unsaturated polyesters or epoxy acrylates. The success of many solvent based and waterborne industrial coatings depends upon the correct amount of cross-linking occurring to give a balance between, for example, the opposing properties of resistance and flexibility. As a general rule, for a given system, the higher the crosslink density, the greater the resistance, but the less the flexibility. There have been great advances in understanding cross-linking, consequently there have been great advances in developing improved cross-linking or co-curing resins, such as aminoplasts or phenolplasts. Another factor driving the thermally cured industrial coating market today is reduced temperature curing systems. This is to reduce energy cost and greenhouse gas emissions. It should not be forgotten that coatings are not only protective and decorative, but they can play a major role in the fabrication or filling of articles. For example, some can coatings are used to enable cans to be formed through deformation of a flat sheet. Can coatings also impart the mobility to beverage cans to allow them to be filled at up to 2,000 cans per minute. As the speed of fabrication or filling increases, so the technology of the coating needs to be changed. In some cases this, way be a minor modification such as changing an additive, but in others it may necessitate the adoption of a new technology.
Coatings can be applied to many articles per minute, as m beverage can coatings with up to 2,000 cans being made and coated per line per minute, or one article over several days or weeks as in the heavy duty coatings for the hold of a ship or oil. rig. Industrial coatings have to be formulated for their conditions of use. Arguably, more sophisticated systems can be used under factory conditions than by a semi skilled person painting an oil rig under adverse weather conditions in the North Sea. Many systems, such as powder, radiation curable and thermally cured ones, can only be applied satisfactorily under factory conditions and for the best and reproducible results, these conditions have to be carefully and rigorously controlled. In this set of books the chemistries of different types of resins for surface coatings are explained. Radiation curable coatings is the subject of a separate series of books. For the reader interested in more detailed information, there are books dedicated to each class of resin.
PAINT TECHNOLOGY – SOME IMPORTANT FACTORS
Dr PKT Oldring
Chapter I I
Before discussing the different technologies employed in the various categories of resins, it may be useful to the reader to discuss some important points of basic paint technology common to all the resins referred to in the chapters of this series of books. The first two sections refer to testing or quantifying the performance of wet and dry paint films and the third discusses paint application techniques. There is also a section briefly discussing the pigmentation of paints. II
PRINCIPAL TESTS FOR PALM AND PAINT FILMS.
The paint industry has a series of tests enabling the testing and evaluation of paints, all of which are part of the readily accessible DIN standards. Those which are commonly used will be discussed, in order to helps formulators with their selection. 1.
Tests on liquid paints.
Measurement of the fineness-of-grind.
This test is carried out with a fineness-of-grind gauge, which is made up of a polished metal plate with 2 grooves whose depth varies uniformly from nothing to a set depth. By depositing a little paint spread over the entire surface, one can determine, during the first five seconds of the measurement the fineness-of-grind of the paint. This is the point at which, surface imperfections (bits) can be first observed. The gauge is marked and the point at which the bits are first seen is read from the gauge. This will give an indication of die gloss and the surface, appearance of the applied and dry paint film, and the resistance to settlement of the liquid paint prior to application. The gauge is cither calibrated in microns or 'Hegman numbers', after the originator. The US uses Hegman numbers, the Europeans microns. The fineness of an undercoat is between 6 - 7 Hegman (30 - 40 im) and a finish or topcoat, 8 - 10 (20 to 1 ìm) (ii)
Measurement of the viscosity.
The paint industry uses metal containers (flow cups) with an. orifice (diameter varying between 1.5 - 6 mm) at their lowest point for the determination of the viscosity of a paint. The efflux (flow) time (normally in seconds) for a fixed volume of paint at a fixed temperature is a useful, simple measurement to compare flow properties of paints, typically at application viscosities. This method is only valid for paint which have little or no thixotropy i.e. Newtonian flow. In Table 1-1 flow times for various standard flow cups commonly employed in the European paint industry, compared with a dynamic viscosity approach. All values are at 20°C.
TABLE 1-1: FLOW TIME IN SECOND Viscosity in mPa
Ford 4 cup AFNOR 4 cup DIN 4 cup
20 25 30 40 50 60 70 80 90 100 120 140 160 180 200 220
10 12 14 18 22 25 28 30 33 35 40 44 50 54 58 62
12 14 16 20 25 29 32 34 37 40 45 50 56 61 66 70
11 12 14 16 20 23 25 26 28 30 34 38 42 45 49 52
Below are listed some typical viscosities which paints would be adjusted to (thinned) prior to application by the mentioned application techniques (AFNOR 4 cup): Brush application Spray gun application Electrostatic application Dipping
60-100s 20-45s 20-30s 25-40s
It should be noted that there are other viscosity measurement techniques. The flow cup is one of the simplest methods. Examples of other techniques are rotating spindle, such as Brookfield, rotating concentric cylinders and cone and plates. Refer to Vol. VI Test Methods for UV & EB Curable Systems by Dr. Chris Lowe, SITA Technology 1998, ISBN 094 7798 072 for further information.
Tests on wet paint films.
Measurement of drying time.
Three types are noted here. (In each case the three parameters which have to be controlled and recorded are temperature, humidity and paint film thickness). (a)
Drying is evaluated by placing grit of a well-defined size onto a freshly. applied film of paint. After a period of time, a brush goes over the paint film in order to see whether the film retains the grit or not. Drying corresponds to the drying time necessary for the grit to stick to the film no longer. (b)
Touch Dry: (or handling ability).
This is the time for which a cigarette paper placed on the paint film (and subjected to a weight of 400 g) can become detached under the action of its own weight, by just turning the film over. A commonly used, but subjective, alterative method for assessing touch dry times is by touching the paint periodically with one's thumb. An anti-corrosion primer will have a touch dry time of 10 to 20 minutes whereas a typical DIY gloss paint will take around 3 hours. (c)
This is the time of drying of the film after which a metallic sheet placed on the film and subjected to a pressure of 0.4 bar, over 10 minutes, leaves no trace on the paint film. It is therefore the time after which the paint will be capable of coping with normal working, handling and storage conditions. There are alterative methods for measuring dryness. There are various pieces of test equipment available to measure surface and through drying. One such common piece of equipment is the BK recorder. The principle is that a weighted needle is slowly propelled through the wet film of paint at a constant rate. This leaves a visible trail in the wet film. As the paint dries, so the trail starts to disappear. When fully dry no sign of the track of the needle remains. The distance related to time for the partial and complete disappearance of marks is a measure of the drying time. 3.
Tests on dry paint films.
The most frequent tests are: measurements of thickness, hardness, impact resistance, stamping, adhesion, resistance to traction tear, resistance to abrasion and scratching, measurement of colour, gloss and orange peel.
This test is carried out using a Persoz or Koenig pendulum and gives a measure of the hardness properties associated with the through film and not just the surface. The oscillations of a pendulum supported by the film (by two steel beads) are more or less dampened depending on the hardness of the film- The hardness is expressed in seconds. Examples of maximum Persoz hardness on aged paint films follow: Chlorinated rubber: Nitrocellulosic: Vinylic: Silicones: Baked alkyds: Baked acrylics: Baked epoxides: Polyurethanes: Glass reference:
120-130 s 120 s 130-150 s 130-150 s 160-180 s 280-320 s 280-300 s 250-300 s 420 s
(It is always necessary to measure this at the same time as the paints and to quote for comparison) (ii)
The resistance of the film of paint to the impact of a 1 kg mass at varying heights can be determined. The mass is placed in a tube which guides its fall. This test is carried out on the painted substrate side (direct impact) or on the reverse side (reverse impact), which is the tougher test. The result is given in cm and corresponds to the minimum height from which flaking (or cracking) in the film of paint can be observed. The test may be slight1y refined by quoting two values, the first is where cracking is first observed but the coating still adheres to the substrate. The second value is for cracking and flaking, when the coating begins to lack adhesion. (iii)
Grid or cross-hatch adhesion test.
The aim of this test is to monitor the adhesion of a film of paint on a given substrate and to Check the interlayer adhesion of a multilayer system. By using a multi-bladed cutting object, a grid is made by drawing it over the paint film and then in a direction at right angles. This results in small squares of approximately 1 mm2 being formed. An adhesive tape, (typically Sellotape), is applied to the scored film and then removed in a rapid but controlled movement. The score of this test is evaluated as a function of pre-established values and ranges from 0 (excellent) to 5 (the area of paint removed represents significantly more than 35 % of the grid area).
Using a pencil holder, the point of the pencil is applied at an angle. of 30' with a 30Og force on the paint film. The instrument is removed and the surface is examined. Failure is at the point at which a pencil, (10H, 9H, 8H, H, F, B, 6B, soft) which has scratched the surface. (v)
Measurement of gloss.
The measurement of specular gloss is carried out using a reflectometer which measures the reflection of a light beam falling onto the film of paint at a specified angle of incidence. 20° angle for high gloss coatings 60° angle for medium gloss coatings 85° angle for matt surfaces Using the general 60° meter the following values would be typical: Absolute gloss Gloss Average satin finish Matt satin finish Matt
= 100 % = 70-85 % (D1Y gloss alkyd = 85%) = 20-30 % = 10-20 % = 0-5 %
Gloss is expressed as a percentage of light retransmitted. (vi)
Exterior exposure (weathering).
Of particular importance to the paint industry is the period during which a paint film will retain its gloss and integrity. Of course, it can be decided by exposing the paint film to the elements, but that will require several years wait hopefully! Therefore the paint industry has devised several accelerated tests to predict the longevity of a Paint film as far as resistance to loss of gloss is concerned. The correlation between the accelerated result and real time weathering varies with the nature of the resin system used and results are interpreted with caution. Xenon lamps and frequent water sprinkling weatherometers are quoted as equating to 1500 to 2000 hours exposure with 2 to 3 years' external natural exposure. During this test, the loss of gloss and change in colour are regularly evaluated. There is also the QUV cabin^ where resistance to UVA and/or UVB radiation interspersed with condensation cycles are used until film destruction occurs. For this particular test, alkyd resins perform poorly as UV radiation wavelengths destroy the resin. This test is high1y controversial since the transmitted UV dose is very high compared to reality and it is difficult to find a relationship between 1000 hours of QUV and natural exposure, such as in Florida, for example.
The evaluation of corrosion resistance remains one of the more important tests for some sectors of the coating industry. The resistance of a film of paint is evaluated by exposing it to a marine atmosphere in a closed cabinet. This atmosphere is achieved using a 5% brine solution. The cabinet is heated to 35'C. This is the well known ASTNI B 117 Accelerated Salt Spray Resistance test. A film of paint is deposited at the required film thickness on the substrate of interest and allowed fully to dry or cure. The painted panel is usually scribed with a cross, which penetrates the paint film through to the substrate, running from the four comers of the panel. The panel is then placed at an angle to the salt spray in the cabinet. Corrosion resistance is evaluated by measuring the density of the pinholes which appear, the blister area, the corrosion creep from the scribe and the loss of gloss. Scales are available which enable a score to be allocated after a certain number of hours of salt spray exposure. Every day, a paint formulator somewhere is working on a project to develop a coating with 250 or 500 hours of salt spray resistance, in addition to the other film attributes desired. III
PAINT APPLICATION METHODS.
To a paint chemist, formulating the paint for film performance properties is only half the job. The other, and arguably more difficult part is to formulate for the application technique that is to be used to apply the paint. Many methods for painting different substrates under various conditions and constraints have been developed, and the choice of the application method depends on many factors. Some key ones are listed below: • • • •
The geometry of the article(s) to be painted, their weight, dimensions and composition. The type of paint (liquid or powder). The rate at which the parts are to be painted. The cost of the painting process. Safety and pollution considerations.
Some of the more common application techniques are discussed below: 1.
Brushes and rollers.
These simple application methods are still used in industry for painting heavy, bulky objects or those for which access is difficult, for examples the holds of 'ships. The brush method offers the advantage of good penetration into all areas of roughness or accessibility of the substrate - particularly important when applying an anti-corrosion primer. A roller does not offer quite the same advantages although a more even paint film thickness can be achieved with automatic airless feed rollers. Both techniques remain rather slow and offer little flexibility with regard to today's economic constraints. Of course, for household decorative paints, the brush and roller are the principal application tools, whether it be for the professionals or DM During paint application to a wall, a roller gives rise to a shear rate of 10,000 s-1 enabling good spreading, flow and substrate wetting.
But, once applied, the paint will have to rapidly adopt a certain structure so as not to sag or run from the wall. To minimise sagging or running, thixotropic alkyds are used which allow the paint to flow under shear and for a certain period after the shear is removed, to allow levelling, but then a rapid increase in viscosity occurs to prevent sagging and slumping. Naturally, the degree of thixotropy is adjustable to anow for the desired amount: of flow and levelling. For example, for a finish and a high build primer Finishing gloss paint → weak thixotropy High build primer → strong thixotropy 2.
There are variations on spray techniques, some of which are described below. Spray application is ideally suited to rapid application of large volumes of paint. (i)
This is the most frequently employed application method in industrial finishing. It is cheap and easy to use. The principal disadvantage is the paint and solvent overspray which needs to be removed continuously with appropriate extraction. Fully extracted water backed spray booths are usually used to cope with this. The paint ed for spray guns may be gravity or pressure pot. (ii)
In this technique, air is no longer used to atomise the paint. The paint is fed at a very high pressure, typically 200 bar, through a fine nozzle or spray tip. The sudden drop in pressure causes the paint to atomise. This system necessitates a high-pressure pump, such as a piston or one of the membrane (diaphragm) types. A number of versions are available, depending on the final use (small or large ratio, hot application paints, two component paints). The airless process brings the following advantages: Total elimination of overspray mists. High throughput and thick coats after one coat. Possibility of applying very heavy paints. On the other hand, this remains a dangerous process and the paint formulation demands are very specific. Airless spraying also yields a relatively poorly atomised paint and thus lay down and flow are often impaired. However, the technique is ideally suited for many applications and is very widely used in heavy duty paint sectors such as marine and maintenance coatings. (iii)
This type of spraying enables practically overspray mist-free paint application and better atomisation, a combination of the advantages of the first two methods. The paint which is ready to spray is pumped to the nozzle by means of a low pressure pump (35 bars) and
atomisation is assisted with a light air stream (1.5 bars). The reduction of misting is due to the slow particle speed (around 0.6 ms- l). This process has the following advantages: Economical in terms of paint, solvent and compressed air. Reduced misting and hence reduced pollution. (iv)
This process consists of giving the paint particles a negative electrical charge which, once placed in an electric field, will be attracted to the earthed part. Figure 1-1 is a schematic representation of an electrostatic spray set up.
Figure 1-1: Schematic representation of an electrostatic spray set up. The advantages and disadvantages of this technique are summarised in Table 1-1 TABLE 1-2: THE ADVANTAGES AND DISADVANTAGES OF ELECTROSTATIC SPRAYING Disadvantages Advantages Cavity coating difficult (Faraday 20 - 30% more efficient compared cage effect) with traditional spraying Need for special solvent to lower Coatings of sharp edges and resistivity hidden corners Easy to automate Article to be painted must be an Possible application of waterelectric conductor dilutable paints The existing equipment can be classified into two types: • Electrostatic guns. • Rotating disc or bell appliances. Rotating bell appliances spray due to the high speed of rotation (40-,000 to 70,000 rotations per minute) of a disc or bell mounted on a compressed air turbine.
These are connected to a high tension generator. The paint flow rates are around 0.4 litres min-1. Transfer efficiencies are very high, rivalling those of powder coatings. (v)
Comparison of different spray application techniques. In Tables 1-3 and 1-4 different spray techniques are compared.
All these processes may have the option of a hot mode whereby paint heated to 60 80'C is applied. This variant offers the following advantages: • • • •
Savings on thinners and time. Thicker layer deposited per coat (higher solids). Shortened dry time - less solvent to evaporate and higher temperature for flash off. Reduced VOC’s.
In the case of alkyds, only those which are non or poor drying can be used, otherwise oxidative cross linking will occur during application. 3.
Immersion Painting (Dipping).
This technique is often used in industry, and involves immersing the articles to be painted in a bath containing the paint. The thickness of the film and the regularity of the deposited coat both depend upon the: • • •
Viscosity and the rheology of the pain Rate of evaporation of the solvents. Immersion rate and shape of the parts.
Practically all types of paints can be used, except two component ones. The bath can be regenerated by regularly adding "fresh" paint. The articles to be painted should have a rather simple geometry. Colour change is obviously to be avoided. The value of the volume of paint in dip tanks is high. 4.
This is a process which is a hybrid of the dip and gun methods. The part to be painted is introduced into a closed vessel and is sprinkled by a large amount of paint mist. Excess paint is recycled after filtration. The installation is rather costly and not very flexible with regard to changes in colour. 5.
Curtain coaters are especially used in the wood industry for coating large fiat areas at a rate of 1 to 2 m/s. The part passes under an extended hopper with an adjustable slit which regulates the rate at which the paint is applied. The amount of product deposited varies from 100 to 300 g/m2. 6.
In this process, the coil of steel is unrolled and passes through two or more rollers impregnated with paint. The coating rates are very high, varying between 60 and 150 min-1. The steel sheet passes through a high temperature oven where the paint is dried and then cooled and recoiled. The coated coil of steel is then used to fabricate articles such as washing machines which are therefore pre-painted. The flexibility requirements of the coating are obviously extremely high. In Table 1-5 the transfer efficiencies of the different application methods are compared. TABLE 1-5: COMPARISON OF THE EFFICIENCIES OF DIFFERENT APPLICATION TECHNIQUES. Application method Pneumatic Airless Electrostatic Electrostatic airless Bell or disc Dipping Coil Coating Electro-deposition (cationic)
% paint deposited on the substrate 35-50 40-65 60-70 45-80 80-90 70 ~80 85-90 90-98
Used for alkyds or polyesters Yes Yes Yes Yes Yes Yes Polyester No
This method of applying coatings is very specialised. There are two classes of electrodeposition paints (electro-paints), namely, anodic: and cathodic. The original electro-paints were anodic, whilst cathodic paints are a more recent development (since the early 80's). Today, for the more demanding applications, such as automobile primers, cathodic electrodeposition is used, due to the better corrosion results obtained. However, for some limited, and often non-critical applications, anodic electro-deposition is still used. Anionic: electro-deposition results in inferior corrosion resistance for two main reasons, which cationic electro-deposition overcomes. Anionic polymers contain carboxyl functionality, which creates an acidic environment which can facilitate corrosion of iron in the presence of moisture. Furthermore, anionic oxidation of steel during electro-deposition creates sites of corrosion. The article to be painted acts as an electrode. It is immersed in a bath containing the coating or paint. Another electrode is in the bath and a current is passed. The paint particles carry the charge and are deposited onto the substrate. This ensures 'hard to reach' parts of a complex shaped object can be painted, for example, an automobile chassis. When the paint film reaches a certain thick-ness it acts as an insulating barrier and no longer conducts electricity at that coated part. Paint is then deposited to other parts which have not yet reached this film thickness. This method ensures that a uniform film is applied over the whole of the object. The paint is, obviously, waterborne. Normally the non-volatile content of an electrodeposition bath is low (15-20%). The voltage, current, time, temperature of bath and nature of the paint all determine the film weight applied. This technique can only be used for the first coating applied and the article to be coated has to be an electrical conductor. Colour change is difficult, due to the large volumes of the electro-deposition tanks. B ath stability is also important. This method of application is ideally suited to production lines, such as automobiles and central heating radiators. Some advantages and disadvantages of electrodeposition are summarised below. Advantages • Ideally suited for automation on a production line. • Uniform film weight applied. • Consistent film weight applied to every article coated, which gives good q. control. • Excellent penetration of hard to reach parts of a complex shaped article. • Fast. • Excellent corrosion resistance possible. Disadvantages • Articles to the coated must be electrical conductors. • High capital investment required. • Potential effluent problems due to low solids. • Limited colour changes. • Need high throughput of articles of the same type. • Changing the article to be coated may require the bath settings to be altered.
EFFECTS OF PIGMENTS AND RILLERS ON FILM PERFORMANCE.
Pigments and fillers used in the paint can provide: • A decorative function. • An anticorrosive function. • Mechanical, chemical or rheological functions. • An extending or cheapening function.
For decoration and opacifying purposes, coloured pigments are used, which can be: • Dye stuffs. • Inorganic and organic pigments. Dye stuffs include natural or synthetic substances, which are soluble in the suspension media and which have zero or very weak opacity. Organic pigments are generally made up of metallic salts with good to moderate opacity. They are bright and transparent and their resistance to degradation in light is variable. Inorganic pigments such as titanium dioxide, red and yellow iron oxides have excellent opacities and are stable (or can be stabilised) in light. Both the organic and inorganic pigments are insoluble in the paint medium or solvents. The choice of pigment or colorant will be based on the following considerations: • Colouring and opacifying ability. • Stability to light, temperature and weathering. • Compatibility with resins. • Price. Table 1-6 lists the majority of organic and inorganic pigments used in paints.
TiO2 anatase TiO2 rutile Lithopone Zinc oxide Iron oxides Graphite Ultramarine blue Prussian blue Cobalt blue Chrome oxide Lemon chrome Medium chrome Orange chrome Cadmium yellow
Iron oxide yellow Molybdenum ORANGE Cadmium red RED Red iron oxide VIOLET Manganese violet Cobalt violet Iron oxide BROWN Sienna Carbon black BLACK Animal black Phthalocyanine BLUE Indanthrone Phthalocyanine GREEN Azoic nickel Flavanthrone YELLOW Benzidene Isoindoline Quinacridone RED Thio indigo Naphtol Toluidene Perilene Alizarine BROWN
VG = Very good
G = Good
VG VG P A
VG VG P G A
VG VG VG P P VG P VG A VG VG VG VG VG VG G * * VG VG *
VG VG P P * VG P VG P VG G G G
VG VG VG G P VG A VG VG
G VG G VG * A VG VG VG P P P A
* * * * P * A A VG VO *
G G G G * VG A p G G P
G G P P * VG A A G G P P
* VG * *
* VG * VG VG A A VG * P G
VG VG VG VG VG VG VG VG
VG VG G
* * VG *
A = Average
Use in interior Most used as Under coat Used in anticorrosion Antirust, Anti acid, Anti acid,
Darkens readily Darkening tendency Does not darken
Heat Resistance Base Resistance Acid Resistance Solvent Resistance Weathering Resistance
TABLE 1-6: INORGANIC AND ORGANIC COLOUR PIGMENTS
Contains sulphides VG
G G VG
P P G
G G VG
G G G
VG VG VG VG VG VG
VG VG VG
G * * * VG *
* VG VG * VG P
P = Poor
G P VG * VG
VG * VG
VG VG P VG
* = Possible Use
Pigments used in anti-corrosion primers play a particular role. These can be divided into: • Anodic protection pigments (chromates and phosphates). • Metallic: pigments providing cathodic protection (zinc or lead). • Inert pigments: these act by the formation of thick lamella structures. They are barriers to water (aluminium, talc, graphite and mica). For information purposes, Table 1-7 lists many commonly used anticorrosion pigments TABLE 1-7: SOME COMMONLY USED ANTI-CORROSION PIGMENTS Material Actirox Anticor Alcophor Bayerferrox Butrol Diroval Delaphos Ferrinox Halox Hispafos Heucophos Heucosil Jacor K WIIITE MOLY WHITE Nalzin Oncor Novinox Phosphìnal Phosphinox Precor Schieldex sicor Strontium chromate AT ZEOLEX Zinkphosphat Zinkoxyd Zinkchromat Wacor ZBP
Supplier Colores Hispania Bayer Henkel Bayer Buckmam Plússtaufer Isc alloys SNCZ Lawrence industries Colores Hispania Heubach Heubach CSF Teíkoku PMC NL Chemical wrnn 5 SNCZ SNCZ SNCZ CSF Grace BASF Habich Zeofmn Oy SNCZ Lehnwm Voss BASF Waardals
Inorganic fillers can do more than just act as a low cost filling material. They can also improve certain properties of the coating. They can be classified according to their chemical and physical properties. (i)
Tale is a magnesium silicate with a hardness equal to 1, with terminal hydroxyl groups and a large specific surface area. The latter point explains the higher quantity of resin than expected required to completely wet out a given amount of tale. (The requirement to entirely wet out the surface of a pigment or filler with a resin in a paint formulation is self evident. Each pigment or filler has a value referred to as its 'oil absorption' and that is determined by the amount of linseed oil required to completely wet out 100g of pigment or filler. The value of oil absorption varies with pigment or extender, for example the oil absorption of titanium dioxide pigment is 20 and the value for a fumed silica extender is around 200.) Talc is insoluble in acids and remains one of the most widely used fillers in alkyd resins. Chlorite is similar to talc. Some of the magnesium is replaced by aluminium in the crystal lattice, giving rise to thicker flakes. The high hydrophobicity of talc imparts a high impermeability to the system towards water and prevents swelling. In solvent systems, its incorporation is easy but in water-dilutable systems, the use of wetting agents is imperative. All lamella products and, in particular, tale, influence the rheological behaviour of the paint. This structure is certainly due to the formation of hydrogen bonds between the resin and the hydroxyl groups of the talc. However, a true thixotropic structure will never be obtained through this system, it is a structured effect. (ii)
Mica is generally used as its Potassium derivative termed moscovite which corresponds to flakes which can undergo bending. During grinding these yield fine flakes of large dimension and hardness (2.5). Mica is chemical and weathering resistant. Plastorite is a type of Mica blended with quartz and chlorite, in a sandwich structure. 1 t is elastic (Mica) to flexible (chlorite), and weathering as well as heat resistant. Plastorite has a smaller specific surface area than talc, which is translated through a lower oil absorption. One can thereby formulate with a higher density concentration of pigment, which is found to be economically favourable. With this filler, a better adhesion on inorganic substrates than with talc or mica is also observed. In the case of talc, a more rapid sedimentation upon storage is also noticeable. (iii)
Kaolin (china clay) is a hydrated aluminium silicate, with yellowish colour and hardness 1.5. (iv)
Carbonates are fillers with a cubic structure whose principal asset is their weak self colour and their good compatibility with other pigments. They can be used as single extending agents in white and pigmented paint systems, in order to achieve pure tones.
The fineness of the carbonate used determines the quantity of expensive white pigment, TiO2, which can be replaced and therefore enables cost saving in the formulation. In sealants (mastics) and filler coating systems, both carbonates and talc are used in order to improve the sealing properties and sanding ability. Carbonates are also found in low cost anti-corrosion systems. Here, they act as sacrificial pigments., lf there is a corrosion attack, the carbonate goes into solution at the same time as the protons of the acid and thereby buffers them, which reduces the rate of corrosion, at least in its initial phase. Today, the low price of fillers remains one of the important factors in their favour, especially when the price of titanium dioxide tends to rise. A well-conceived formulation enables one also to save costs on pigments as well as additives which remain a lot more expensive. In Table 1-8 the principal fillers used are listed.
Kaolin Mica Tale Pumice Glass bead Colloidal silica Calcite chalk Aluminium paste Graphite Carbon black Aluminium powder Zinc powder
TABLE 1-8: COMMONLY USED PAINT FILLERS
x x x
Effect of the amount of pigment on paint properties.
Pigment by volume concentration (PVC).
x x x x
Research has shown that the properties of a paint depend essentially on the ratio of the volumes of the pigments and fillers used and the volume of the dry film. Therefore a most useful calculation is given by the concentration of pigment by volume or PVC. The pigment volume concentration is defined as the fractional volume of pigment (including fillers) in a unit volume of a given pigment binder mixture.
PVC = VP/(VP+Vb) WhereVp = volume of pigments and filler, Vb = volume of binder, volatiles excluded. It follows that as the PVC of a paint film increases, a point will be reached when the pigment and filler particles have effectively used up all the available resin for surface wetting and addition of further pigment will result in pigment to pigment contact rather than pigment: to resin contact in the film. This point is known as the Critical Pigment Volume Concentration, or CPVC. The critical pigment volume concentration CPVC, corresponds to the limit beyond which significant modifications in the paint film properties can be observed, such as an increase in permeability of a film to water vapour or a reduction in the resistance to corrosion. The following discussion lists the main trends as a function of the amount of filler expressed as PVC. A very useful concept in paint formulating is to use the function of the pigment volume concentration as a percentage of the CPVC. Note that, beyond a certain PVC/CPVC percentage, a sudden drop in properties occurs. The best results depend on the nature of the pigments but they are generally with the following PVC range: Primers: 30 % < PVC < 50 % (Except for primers with high zinc content PVC > 95%) Intermediate coats: 30 % < PVC < 35 % Finishing coats: PVC < 20 % (ii)
Changes in characteristics as a functions of the amount of pigmentation.
(a) Gloss. Between 20% and 30%, PVC has only a small influence, but thereafter a very sharp fall is found which reaches the start of its asymptote at around 42% of the CPVC which then levels off. (b) Blistering. This parameter starts to decrease above 30% of the CPVC, reaching its minimum at 60%. (c) Corrosion. Corrosion resistance remains very low up to a value of around 42% of the CPVC, and then it strongly increases, reaching its maximum at 55 %. (d) Permeability. This follows the same behaviour as corrosion resistance with a slower evolution. Note the presence of a PVC 'zone' around 45% of the CPVC where all the characteristics cross. This corresponds to a "no-go zone" for the parameters studied. In this zone, almost all parameters are at their minimal level, or conversely the paint formulation is 'optimised'.
by Phillipe Deligny Dr. N. Tuck Edited by Dr. P. K. T. Oldring
For many years, resins resulting from the polycondensation of polyacids and polyols have been used in the paint industry. They have been named in many different ways which have led to ambiguities, as to the composition and utilisation of these products. "Alkyds, Polyesters, Glycerols, Glycerophthalics, Oil-free Polyesters" The term "Alkyds", which is one of the more commonly employed definitions, was created in 1914 by Kienle. It corresponds to the euphonic contraction of the words '1alcohol" and "acid" indicating the polycondensate obtained from fatty acids, polyols and polyacids. The term "Glycerophthalic" arises from the fact that the first resins were based on glycerol and phthalic anhydride. The first attempts at polycondensation were carried out by Belzelius, in 1847, who prepared glyceryl polytartrate, then by Smith, in 1901, who synthesised glycerol polyphthalate. The film-forming property of this product was improved by Kienle (1914) who modified it with natural oil fatty acids. The thereby formed resins were sold by General Electric under the name “Glyptal” However, the real credit for the development of alkyd resins in paints can be given to chemists working in Bayer laboratories (at the time of 1 G Farben) who discovered, in 1927, the transesterification process of oils which enabled the direct use of these oils as basic components without having to use fatty acids. This process enabled the development of the range of "Alkydal" resins for paints. In this chapter alkyd resins will be considered as those which result from the polycondensation of polyols with polyacids and for which, at least a part of the polyacids (the most frequent case) will comprise a fatty acid or oil, of natural or synthetic origin, and which will possess either oxidative drying ('drying') or non-oxidative drying ('non-drying') properties. II
Types of alkyds.
Alkyd resins of various oil lengths and degrees of modification are still widely used in industrial and D1Y applications. Below is a discussion of the various types of alkyd, a brief description of their properties and some comments on their suitability for various end uses. It is interesting to note that some oils, precursors for alkyd resins, are still. directly used in paints or for the preparation of certain coatings. For this reason linseed oil is used alone or in stand oils for wood or early anticorrosion primers. China wood (Tung) and Soya bean oils as well as stand oil-based oils can also be found. Lime based oils are still found in matt paints for ceilings for application and brushability reasons, as well as for coating old substrates for either authenticity or preservation purposes.
Long oil alkyds: air drying and aliphatic solvent compatible.
Long oil alkyds, containing >55% of a drying oil, are used in building interiors and D1Y paints, such as matt, satin, gloss finishes, primers and for wood (stains and varnishes). They are stilly widely used in marine and maintenance applications as primers and finishes. Advantages •
Air drying in 5 to 8 hours, low viscosity, excellent gloss, and wetting of pigments. They can be formulated at 100% solids and as emulsions in water. Thixotropic variants can be formulated.
Poor hardness, solvent, alkali and hydrocarbon sensitive, poor exterior resistance. The long oil alkyds can exhibit a tendency to yellowing in darkness, an undesirable feature in white D1Y finishes where areas that are not exposed to light exist next to areas that are, on a window sill for example that may have pot plants. The area under the pot yellows and when the pot is subsequently moved, a yellows area is revealed. The yellowing will eventually disappear, bleached by the light. They are susceptible to specifications, and therefore degrade relatively rapidly.
(ii) Medium oil alkyds: air and oven drying; aliphatic and aromatic solvent compatible. Medium oil alkyds, containing 45-55% of oil, are often used in low cost anticorrosion primers, D1Y paints (especially matt and satin-finish) and some industrial stoving enamels such as for agricultural machinery. Advantages •
Air drying in 3 hours, rather high viscosity, induced or assisted air drying (50 – 80°C), good gloss. They can be used in paints along with long oils to improve metal adhesion of the long oils.
Poor hardness, hydrocarbon, alkali and oil sensitive.
(iii) Short oil alkyds: air and oven drying; aromatic hydrocarbon and ester solvent compatibility. The main application of short oil alkyds, containing